In situ anchoring iron oxide nanoparticles onto polyester/disperse dye for production of multifunctional fabrics
Fashion and Textiles volume 10, Article number: 41 (2023)
Medical textiles, including surgical gowns, masks are used as obstacles to prevent the risk of infection for both doctor and patient. The widespread of bacteria and viruses, e.g. chronic hepatitis B, hepatitis C and currently Covid-19 viruses in the patient population is very common. In this work, multifunctional eco-friendly polyester fabrics have been produced by in situ impregnation of 2-((E)-(2-(2,4-dinitrophenyl)hydrazono)methyl)-4-((E)-phenyldiazenyl)phenol disperse dye onto magnetic iron oxide nanoparticles. The technique endowed polyester fabrics with a new color as well as magnetic and antibacterial functionalities. The colored magnetic nanoparticles showed high affinity toward fabrics. Besides, the unbound dye could be easily collected from wastewater by a magnet, significantly facilitate the wastewater treatment. The treated fabrics were analyzed by energy dispersive X-ray spectroscopy, scanning electron microscopy, X-ray diffraction and vibrating sample magnetometry. Colorimetric values, tensile properties and fastness of the composite fabrics were also measured. The tensile properties of the composite were increased after functionalization. The wettability features of the fabric were investigated and showed a significant improvement. Also, the toxicity of the resulted fabric was exhibited low toxicity against wi-38 cell line. These results indicate the potentiality of the suggested technique in producing multifunctional fabrics with various applications, especially as medical textiles.
Nanomaterials of magnetic elements are known as magnetic nanoparticles (MNPs). It has received an extensive consideration owing to their impressive merits. They have high surface area, superparamagnetic properties, great ability for modification and lower bio-toxicity (Zhang et al., 2017a, b). The most important of this category are iron (Fe), cobalt (Co) and nickel (Ni) due to its high magnetic properties and high ability to control and regulate the size and composition as well as the shape compared to magnetic metal oxide nanoparticles (Hedayatnasab et al., 2017). Recently, iron and iron oxide, especially in its nanosized forms have received significant interest because of their excellent magnetic properties (Jadoun et al., 2020; McCafferty et al., 2015; Sharouf & Saffour, 2023). Moreover, magnetic iron oxide nanoparticles (MIONPs) has been highlighted due to their utilization in adsorption of metal aqua ions like Cu2+, Hg2+, Cr6+, Au3+ As3+ and organic compounds from aqueous solution (Shahidi, 2019; Zhang et al., 2017a, b). Furthermore, iron-based NPs have their own unique properties such as antimicrobial and/or antiviral properties, self-clean, anti UV, wettability which further improve the material finishing (Tan et al., 2019). Accordingly, researchers and scientists have used iron oxide NPs in protective textiles and medical applications for the prevention of microbial and viral infections due to its delightful performance (Abou Elmaaty et al., 2018a, b; Elmaaty et al., 2018b; Hebeish et al., 2015; Ibrahim et al., 2013a, b, c, 2015, 2017a, b, 2018; Shahidi, 2016).
Harifi et al. reported on the utilization of ferric chloride under a sonochemical method to in situ synthesize the hematite and magnetite NPs which further deposited on polyester fabric (Harifi & Montazer, 2014). The resulted fabrics exhibited durable biological activity and magnetic properties which are useful for use in antibacterial and electromagnetic shielding (EMS) applications. Rastgoo et al. (2016) used ultrasound mediation for preparing Fe3O4 on cotton/polyester fabric that showed sonocatalytic, photocatalytic, antibacterial and magnetic characteristics (Rastgoo et al., 2016). As for the removal of dye or other organic compounds; Wen et al. reported that cotton fabrics were dyed with (disperse red 1) with the coloured (MIONPs) suspension by a dip-pad-dry method and after dyeing; wastewater was exposed to magnets. The unattached dyes were collected by magnets and was reused in the next dyeing processes (Wen & Sun, 2018). All previous methods utilized multiple steps to implement the fabrics with the combination of colour and functional properties and consequently suffered from the disadvantages of concomitant consumption of water, chemicals and energy. The present research was directed to develop a novel in situ method to overcome the disadvantages mentioned above by using one-step MIONPs anchoring and dyeing of PET fabric with multifunctional properties. This research also aims to improve the properties of water absorption and dyeing by hydrophobic polyester, in addition to improving the resistance to bacteria. The resulted multifunctional PET fabric is a promising candidate for using as medical textile and in dye removal.
A 100% plain-weave polyester (PET) fabric with wight of 108 g/m2 and it was 70 denier warps and 150 denier weftswas purchased from Omar Afandy Co., Egypt. As for chemicals; ferrous sulfate (FeSO4⋅7H2O), ferric trichloride (FeCl3), sodium hydroxide (NaOH) and dispersing agent were used. The dyestuff used in this study was synthesized according to the method previously reported (Fig. 1) (Dehspande et al., 2012).
In situ dyeing and synthesis of (IONPs) on polyester fabric
The IONPs were synthesized on the polyester fabric by treating the fabric in a bath containing: FeCl3, FeSO4⋅7H2O (Fe2+/Fe3+ molar ratio = 2), NaOH (pH = 12), dispersing agent and azo disperse dye. The liquor ratio was kept at 1:100. The synthesis was conducted at a temperature of 100 °C for 60 min. Finally, the resulted fabrics were rinsed with water for 15 min. at 60 °C and dried at around 20–22 °C. The resulted fabric coded with D/T.
XRD was performed with a Bruker D8 ADVANCE, Karlsruhe, Germany using a Cu radiation source (30 mA) running at 40 kV to explore the crystalline phases and size of IONPs on the polyester fabric. The surface morphology of the D/T fabric and particle size of IONPs were analyzed by using Jeol-Japan-JSM-6510LVscanning electron microscope (SEM). The elemental composition of resulted fabrics was analyzed by using Oxford-x max 20 Energy Dispersive Spectrometer (EDX). The fastness properties of D/T fabric were measured by using methods of AATCC TM 61-1996 ("American Association of Textile Chemists and Colorists, AATTCC 61-1996: Colorfastness to Laundering: Accelerated, Research Triangle Park, NC, USA", 1996), AATCC TM 8-1996 ("American Association of Textile Chemists and Colorists, AATCC Test Method 8-1996, Colorfastness to Crocking, Research Triangle Park, NC, USA," 1996) and AATCC TM 16 .2-2022 ("American Association of Textile Chemists and Colorists. AATCC TM16.2-2022, Test Method for Colorfastness to Light: Carbon-Arc," 2022) for washing, dry/wet rubbing, and lightfastness, respectively. The antibacterial activity of the dyed and D/T polyester fabrics were assessed quantitatively according to AATCC TM 147 -2004 ("American Association of Textile Chemists and Colorists, AATTCC 147-2004: Antibacterial Activity Assessment of Textile Materials, Research Triangle Park, NC, USA," 2010) method against Staphylococcus aureus and Bacillus cereus as a gram-positive bacterium and gram-negative bacterium (E. coli). The magnetization was measured using vibrating sample magnetometry at room temperature. The color strength (K/S) of treated fabric with IONPS was analyzed by using Konica-Minolta-CM-3600A spectrophotometer. Wettability of untreated and D/T fabric was evaluated by calculating the time that takes to absorb one drop of distilled water dropped on the fabric. Moreover, the tensile strength of the untreated and D/T fabrics was measured by using Mecmesin-AFG-1000N instrument for three repeated measurements, and the mean value was taken. AATCC TM 61(2A)-1996 ("American Association of Textile Chemists and Colorists, AATCC 61(2A): Colorfastness to laundering, Research Triangle Park, NC, USA ", 1996) method was used to evaluate the durability after five washing cycles. The uptake of the dye by the polyester fabric was measured by using UV/VIS spectrophotometer-model: Alpha -1860. The toxicity of D/T fabrics was tested according to the MTT assay protocol.
Results and Discussion
Synthesis of iron oxide nanoparticles
As reported previously (Harifi & Montazer, 2014); IONPs were formed after blending the iron salts with sodium hydroxide solution. Where the reactions occurring to form IONPs are as follows (Harifi & Montazer, 2014):
The synthesis procedures take place at high pH value, during which hydroxylation of Fe2+ and Fe3+ species was obtained simultaneously [reactions (1) and (2)] (Hribernik et al., 2012) carrying out the process at boiling for 60 min. This process allowed enough time for the evolution of magnetite (Fe3O4) nucleus to complete. Whereas the average pH for the synthesis of magnetite NPs is ~ 11, (Faiyas et al., 2010). We adjusted the pH at 12, as reported in Faiyas et al. (2010); the evolution of magnetite was carried out at a pH higher than 11. Also, the carboxyl (–COO−) functional group on polymeric chains of polyester fibers was generated in alkaline solution as in the Eq. (4). The iron ions with positive charge can subsequently absorb on negative groups created on polyester fabric by ionic interactions [reaction (5)]. The ionic interactions and hydrogen bonding with functional groups of polymeric substrates were mainly remarked for adsorption of nanoparticles on the surface in nano-functionalization of polyester fabrics (Rezaie & Montazer, 2019).
Cytotoxicity test on D/T fabric
The cytotoxicity of D/T fabric was evaluated against healthy human cells (wi-38) by the MTT assay. Figure 2 and Table 1 show that the viability of cells of D/T fabric was 99.7% of the negative control. However, the average relative cell viability was over 70%, as mentioned in (Kangwansupamonkon et al., 2009), and it was concluded that the D/T fabrics have low toxicity toward human skin. Which leads to the use of these fabrics in the medical fields.
The colour parameters of the dyed and D/T polyester fabrics were analyzed by using the (Konica Minolta spectrophotometer CM-3600A). Figure 3 and Table 2 exhibit the L*a*b* values for each fabric, where (L*) values represent colour lightness, (a*) is the red/green coordinate, and (b*) is the yellow/blue coordinate (Khalifa et al., 2015), we can objectively determine that the fabrics do not match in colour. These values tell us that D/T fabric is darker according to the colour lightness values L*, greener and less blue according to a*, b* values respectively than Dyed fabrics. If we put the values of ΔL* = + 42.28, Δa* = + 3.11, and Δb* = + 58.09 into the colour difference equation, it can be determined that the total colour difference between the two fabrics is ~ 71.9.
Effect of in situ application with different dye concentrations on color strength (K/S)
Figure 4 shows that increasing dye concentration from 1 to 3% (owf) lead to an increase in dye uptake. The maximum K/S value was reached at 3% concentration of the dye. This result referred that by increasing the dye concentration, the dye diffusion into fabrics increased (Elmaaty et al., 2018a). Further increase in dye concentration has no effect on the K/S value. This may be attributed to over saturation of the fabric by dye and NPs (Abou Elmaaty et al., 2020).
Effect of temperature and time of in situ application on color strength (K/S)
The effect of in situ application settings on (K/S values) was investigated. Various temperatures (60, 100, and 130 °C) and durations (30, 60 and 120 min.) were applied on polyester fabrics with dye and IONPs, and the results were shown in Figs. 5 and 6. It can be concluded from Fig. 5 that; raising the temperature from 60 to 100 °C increased the K/S from (9.6 to 17.3), this may be referred to the high distribution rate and the raise of the kinetic energy of the dye molecules. Thus 100 °C was selected as an optimum temperature for the application. Above optimum temperature, the rate of dyeing is reversed, and the dye may not stabilize onto fabrics resulting in reducing the K/S and reducing the fastness properties (Adeel et al., 2018). Otherwise, the maximum K/S value, 17.3 has been recorded after 60 min in Fig. 6. Increasing the application time above 60 min caused a reduction in the K/S values. This result may be referred to the fact that the heating for a long time may cause stripping and equilibrium are favoured towards the treatment bath (Adeel et al., 2018).
Effect of pH on color strength (K/S)
Figure 7 showed that the (K/S) of D/T polyester fabric was increased by increasing the pH value of the treatment bath from pH 5 to 12. The better result and the maximum uptake of dye and IONPs were gained at pH 12. This may be referred to the growth of Fe3O4 nuclei which was occurred at pH higher than 11 (Faiyas et al., 2010). In addition; it can be suggested that the alkaline hydrolysis of polyester causes the formation of polyethylene glycol and through the oxidation of hydroxyl groups to aldehyde groups in ethylene glycol, carboxylate ions was produced. This increases the tendency of fabric surface toward IONPs (Allahyarzadeh et al., 2013).
Figure 8 showed XRD pattern of synthesized IONPs on treated polyester fabrics exhibiting peaks at 2Ɵ at 30.1, 35.5, 42.6, 53.6, 57.0 and 62.8 which can be assigned to diffraction of the (220), (311), (400), (422), (511), and (440) planes, respectively of spinal structured Fe3O4 nanoparticles. Accordingly, we can conclude that the resulted fabric had perfect magnetic responsivity (Xu et al., 2016).
Figure 9 shows the relationship between the applied magnetic field (H) and the induced magnetization (M) of the D/T fabric exhibiting a sharp increase in magnetization by increasing the applied field from 0 to 20 KG.
SEM and EDX analysis
The IONPs were uniformly distributed on the surface of the D/T fabric, as seen in Fig. 10. The synthesized IONPs are 20–28 nm and roughly agglomerated. Figure 11 confirmed the successful synthesis of the IONPs on the D/T fabric by using EDX to analyze the chemical compositions. The figure also showed that iron and oxygen were two elements in the D/T fabric regardless of the carbon that was bound to the polyester substrate.
To determine the antibacterial activity of the D/T fabrics against Staphylococcus aureus and Bacillus cereus as a gram-positive bacterium and gram-negative bacterium (E. coli); the AATCC T M 100-2004 method was used (Test method for antibacterial finishes on textile materials, 2004). And according to Eq. (6); the results were reported as percentages of bacteria reduction.
where R is the reduction percentage of bacteria colonies, A and B are the numbers of bacteria colonies recovered from the blank and D/T fabric, respectively after inoculation and incubation. The antibacterial efficiencies of the D/T fabrics against Staphylococcus aureus, Bacillus cereus and E. coli bacteria were 52, 71 and 15%, respectively as shown in Table 3. The reaction between bacteria and IONPs causes the death of bacteria (Shahidi et al., 2018) as a result of changing the metabolic activity of bacteria. IONPs were promising agents for antibacterial applications (Harifi & Montazer, 2014) due to its unique characteristics. Also; by increasing the iron nanoparticles on polyester fabric the magnetic field increases, which is one of the distinctive characteristics of it, which in turn increases the bactericidal action causing bacteria cell death (Gudkov et al., 2021).
Water drop test
The hydrophobicity of untreated and D/T fabrics was measured by the water drop test. A controlled size drop was placed at a constant rate onto the surface of the fabric, and the time required for penetration was calculated. The uptake times have been taken for untreated and D/T polyester fabrics. It has been found that the time spent to absorb one water droplet on the untreated polyester fabric was 6 s, however this time for D/T fabric reduced to 4 s. The surface wettability of the D/T fabrics was enhanced with minor etching effects as a result of surface oxidation of the D/T fabrics.
Also, Fig. 12 reveals the length of water droplet diameter after absorption and spreading in the time frames that were mentioned before for both fabrics.
By using overall optimum conditions, the durability of D/T polyester fabric was assessed in terms of color fastness mainly washing, rubbing, and light. As seen in Table 4; the wash and rubbing fastness of D/T polyester fabric were excellent and very good, respectively, even after five washing cycles. As for light fastness, moderate values were observed even after five washing cycles. This result may be attributed to the photo fading behaviors of disperse dyes (Suesat & Suwanruji, 2011).
According to the results of the tensile strength (maximum force), which was listed in Table 5, it can be concluded that the introduction of IONP into the structure of polyester fabric improved the tensile strength of the treated fabric, possibly due to the ionic interactions and hydrogen bonding between IONPs and polyester fabric (Rezaie & Montazer, 2019) and due to the filling of any pits that can result from the hydrolysis of polyester by synthesized IONPs resulting in a uniform distribution of load on the fabric surface (Harifi & Montazer, 2014).
Measurement of dye exhaustion
The dyebath solution was sampled before and after dyeing to measure the dye exhaustion. The solution of the dye was diluted 20-fold with 85% aqueous DMF. Moreover, the absorbance of the dye solution was measured by using UV/VIS spectrophotometer-model: Alpha -1860. A calibration curve with known dilution degrees of the dye concentration in 80% aqueous DMF (Fig. 13) was also used. The dye exhaustion is calculated by using Eq. 7:
where (%E) is the percentage of dye exhaustion and C1, C2 are the dye concentrations in the solutions before and after dyeing, respectively. Figure 14 has shown the absorbance of dye bath concentration before and after exhaustion by polyester fabric. The decrease in absorbance is due to the increase of dye exhaustion by polyester fabric, which means that the dye and iron nanoparticles have been absorbed by polyester fabric and the treatment was occurred.
This work discusses a new approach of colouring MIONPs and implementing the fabric with multifunctional properties in one step by using in situ technique. The optimum condition of the treatment has been controlled by adjusting the pH at 12, treatment time for 60min., treatment temperature at 100 °C and IONPs concentration of 3% owf. The results of the SEM, EDX and XRD measurements confirmed the successful synthesis of IONPs with size around of 20–28 nm as well as the uniformty of color distribution on polyester fabrics. Moreover, the colored polyester fabric acquired excellent color fastness properties, their noticeable improve in antibacterial activity against Bacillus cereus (with 71% of reduction of bacterial growth), low toxicity of 0.26% against wi-38 cell line and the increase in magnetization pointed to an eco-friendlier approach in textile dyeing and multifunctionalization. Also, the un-attached coloured magnetic IONPs can be collected, re-concentrated and reused again by using a magnet in a simple, cost-effective, and environmental-friendly way for the wastewater treatment process.
Availability of data and materials
The datasets generated and/or analyzed during the current study are available from the corresponding author on reasonable request.
Abou Elmaaty, T., Abdelaziz, E., Nasser, D., Abdelfattah, K., Elkadi, S., & Elnagar, K. (2018a). Microwave and nanotechnology advanced solutions to improve ecofriendly cotton’s coloration and performance properties. Egyptian Journal of Chemistry, 61, 370–380. https://doi.org/10.21608/ejchem.2018.2927.1270
Abou Elmaaty, T. M., Abdeldayem, S. A., & Elshafai, N. (2020). Simultaneous thermochromic pigment printing and Se-NP multifunctional finishing of cotton fabrics for smart childrenswear. Cloth Tex Res J, 38(3), 182–195. https://doi.org/10.1177/0887302X19899992
Abou Elmaaty, T., Elnagar, K., Raouf, S., Abdelfattah, K., El-Kadi, S., & Abdelaziz, E. (2018b). One-step green approach for functional printing and finishing of textiles using silver and gold NPs. RSC Advances, 8, 25546–25557. https://doi.org/10.1039/C8RA02573H
Adeel, S., Khan, S., Shahid, S., Saeed, M., Kiran, S., Suleman, M., & Akhtar, N. (2018). Sustainable dyeing of microwave treated polyester fabric using disperse yellow 211 dye. J Mexican Chem Soc. https://doi.org/10.1016/10.29356/jmcs.v62i1.580
Allahyarzadeh, V., Montazer, M., Nejad, N. H., & Samadi, N. (2013). In situ synthesis of nano silver on polyester using NaOH/Nano TiO2. Journal of Applied Polymer Science, 129(2), 892–900. https://doi.org/10.1002/app.38907
Dehspande, H., Chopde, H., Pandhurnekar, C., & Batra, R. (2012). Synthesis, characterization and testing of biological activity of some novel chalcones derivatives of coumarin. Chem Sci Trans, 2, 621. https://doi.org/10.1016/10.7598/cst2013.317
Elmaaty, T. A., El-Taweel, F., Elsisi, H., & Okubayashi, S. (2018a). Water free dyeing of polypropylene fabric under supercritical carbon dioxide and comparison with its aqueous analogue. Journal of Supercritical Fluids, 139, 114–121. https://doi.org/10.1016/j.supflu.2018.05.018
Elmaaty, T. A., Ramadan, S. M., Nasr-Eldin, S. M., & Elgamal, G. (2018b). One step thermochromic pigment printing and Ag NPs antibacterial functional finishing of cotton and cotton/PET fabrics. Fibers Polym, 19, 2317–2323. https://doi.org/10.1007/s12221-018-8609-x
Faiyas, A. P. A., Vinod, E. M., Joseph, J., Ganesan, R., & Pandey, R. K. (2010). Dependence of pH and surfactant effect in the synthesis of magnetite (Fe3O4) nanoparticles and its properties. Journal of Magnetism and Magnetic Materials, 322(4), 400–404. https://doi.org/10.1016/j.jmmm.2009.09.064
Gudkov, S. V., Burmistrov, D. E., Serov, D. A., Rebezov, M. B., Semenova, A. A., & Lisitsyn, A. B. (2021). Do iron oxide nanoparticles have significant antibacterial properties? Antibiotics (basel). https://doi.org/10.3390/antibiotics10070884
Harifi, T., & Montazer, M. (2014a). In situ synthesis of iron oxide nanoparticles on polyester fabric utilizing color, magnetic, antibacterial and sono-Fenton catalytic properties. J Mater Chem B, 2(3), 272–282. https://doi.org/10.1039/c3tb21445a
Hebeish, A., Abou Elmaaty, T., Ramadan, M., & Magdy, H. (2015). Microwave and plasma treatments for functionalization of polyester fabrics. Int J Curr Microbiol Appl Sci, 4, 703–715.
Hedayatnasab, Z., Abnisa, F., & Daud, W. M. A. W. (2017). Review on magnetic nanoparticles for magnetic nanofluid hyperthermia application. Materials and Design, 123, 174–196. https://doi.org/10.1016/j.matdes.2017.03.036
Hribernik, S., Sfiligoj-Smole, M., Bele, M., Gyergyek, S., Jamnik, J., & Stana-Kleinschek, K. (2012). Synthesis of magnetic iron oxide particles: Development of an in situ coating procedure for fibrous materials. Colloids and Surfaces, a: Physicochemical and Engineering Aspects, 400, 58–66. https://doi.org/10.1016/j.colsurfa.2012.02.052
Ibrahim, N., Abd El-Aziz, E., Eid, B., & Abou Elmaaty, T. (2015). Single-stage process for bifunctionalization and eco-friendly pigment coloration of cellulosic fabrics. J Tex Inst, 107, 1022–1029. https://doi.org/10.1080/00405000.2015.1082784
Ibrahim, N. A., Eid, B. M., Abd El-Aziz, E., & Abou Elmaaty, T. M. (2013a). Functionalization of linen/cotton pigment prints using inorganic nano structure materials. Carbohydrate Polymers, 97, 537–545. https://doi.org/10.1016/j.carbpol.2013.04.084
Ibrahim, N. A., Eid, B. M., & Abdel-Aziz, M. S. (2017a). Effect of plasma superficial treatments on antibacterial functionalization and coloration of cellulosic fabrics. Applied Surface Science, 392, 1126–1133. https://doi.org/10.1016/j.apsusc.2016.09.141
Ibrahim, N., Eid, B., Abdellatif, F., & Yusuf, M. (2018). Advanced materials and technologies for antimicrobial finishing of cellulosic textiles. Handbook of renewable materials for coloration and finishing (pp. 301–356). https://doi.org/10.1002/9781119407850.ch13
Ibrahim, N. A., Eid, B. M., El-Aziz, E. A., Abou Elmaaty, T. M., & Ramadan, S. M. (2017b). Multifunctional cellulose-containing fabrics using modified finishing formulations. RSC Advances, 7, 33219–33230. https://doi.org/10.1039/C7RA05403C
Ibrahim, N. A., Eid, B. M., Elmaaty, T. M. A., & El-Aziz, E. A. (2013b). A smart approach to add antibacterial functionality to cellulosic pigment prints. Carbohydrate Polymers, 94, 612–618. https://doi.org/10.1016/j.carbpol.2013.01.040
Ibrahim, N., Elmaaty, T. A., Eid, B., & El-Aziz, E. A. (2013c). Combined antimicrobial finishing and pigment printing of cotton/polyester blends. Carbohydrate Polymers, 95, 379–388. https://doi.org/10.1016/j.carbpol.2013.02.078
Jadoun, S., Verma, A., & Arif, R. (2020). Modification of textiles via nanomaterials and their applications. Frontiers of textile materials (pp. 135–152). Wiley. https://doi.org/10.1002/9781119620396.ch6
Kangwansupamonkon, W., Lauruengtana, V., Surassmo, S., & Ruktanonchai, U. (2009). Antibacterial effect of apatite-coated titanium dioxide for textiles applications. Nanomedicine: Nanotechnology, Biology and Medicine, 5(2), 240–249. https://doi.org/10.1016/j.nano.2008.09.004
Khalifa, M. E., Abdel-Latif, E., & Gobouri, A. A. (2015). Disperse Dyes Based on 5-Arylazo-thiazol-2-ylcarbamoyl-thiophenes: synthesis, antimicrobial activity and their application on polyester. Journal of Heterocyclic Chemistry, 52(3), 674–680. https://doi.org/10.1016/10.1002/jhet.2153
McCafferty, L., Stolojan, V., King, S. G., Zhang, W., Haq, S., & Silva, S. R. P. (2015). Decoration of multiwalled carbon nanotubes with protected iron nanoparticles. Carbon, 84, 47–55. https://doi.org/10.1016/j.carbon.2014.11.042
Rastgoo, M., Montazer, M., Malek, R. M. A., Harifi, T., & Mahmoudi Rad, M. (2016). Ultrasound mediation for one-pot sonosynthesis and deposition of magnetite nanoparticles on cotton/polyester fabric as a novel magnetic, photocatalytic, sonocatalytic, antibacterial and antifungal textile. Ultrasonics Sonochem, 31, 257–266. https://doi.org/10.1016/j.ultsonch.2016.01.008
Rezaie, A. B., & Montazer, M. (2019). Surface functionalization of polyester fibers via one-step green formation and assembling of iron oxide nanoparticles with photo and magneto activities. Fibers Polym, 20(5), 951–960. https://doi.org/10.1007/s12221-019-9046-1
Shahidi, S. (2016). Antibacterial efficiency of mordant-treated cotton and polyamide fabrics, before and after dyeing. J Nat Fibers, 13, 507–519. https://doi.org/10.1080/15440478.2015.1066290
Shahidi, S. (2019). Magnetic nanoparticles application in the textile industry—a review. J Ind Tex. https://doi.org/10.1177/1528083719851852
Shahidi, S., Mazaheri, F., Moazzenchi, B., & Hoseini, H. (2018). Studying the magnetic, antibacterial, and catalytic activity properties of DBD/iron oxide nanoparticle-treated cotton fabric. J Nat Fibers, 15(5), 731–739. https://doi.org/10.1080/15440478.2017.1361372
Sharouf, H., & Saffour, Z. (2023). Synthesizing and using iron oxide nanoparticles as nanocomposite in cotton fabrics nanofinishing. Baghdad Science Journal. https://doi.org/10.21123/bsj.2023.7743
Suesat, J., & Suwanruji, P. (2011). Dyeing and fastness properties of disperse dyes on poly(lactic acid) fiber. InTech. https://doi.org/10.5772/23126
Tan, L.-Y., Sin, L. T., Bee, S.-T., Ratnam, C. T., Woo, K.-K., Tee, T.-T., & Rahmat, A. R. (2019). A review of antimicrobial fabric containing nanostructures metal-based compound. Journal of Vinyl & Additive Technology, 25(S1), E3–E27. https://doi.org/10.1002/vnl.21606
Test method for antibacterial finishes on textile materials. (2004). American Association of Textile Chemists and Colorists. AATCC 100–2004, Research Triangle Park, NC, USA.
Wen, J., & Sun, Y. (2018). Colored magnetic nanoparticles to improve the sustainability of textile dyeing. TechConnect Briefs, 2, 245–248.
Xu, M., Liu, M., Sun, M., Chen, K., Cao, X., & Hu, Y. (2016). Magnetic solid-phase extraction of phthalate esters (PAEs) in apparel textile by core–shell structured Fe3O4@silica@triblock-copolymer magnetic microspheres. Talanta, 150, 125–134. https://doi.org/10.1016/j.talanta.2015.12.027
Zhang, J., Shao, Y., Hsieh, C.-T., Chen, Y.-F., Su, T.-C., Hsu, J.-P., & Juang, R.-S. (2017a). Synthesis of magnetic iron oxide nanoparticles onto fluorinated carbon fabrics for contaminant removal and oil-water separation. Separation and Purification Technology, 174, 312–319. https://doi.org/10.1016/j.seppur.2016.11.006
Zhang, Z., Guan, Y., Xia, T., Du, J., Li, T., Sun, Z., & Guo, C. (2017b). Influence of exposed magnetic nanoparticles and their application in chemiluminescence immunoassay. Colloids and Surfaces, a: Physicochemical and Engineering Aspects, 520, 335–342. https://doi.org/10.1016/j.colsurfa.2017.01.071
Open access funding provided by The Science, Technology & Innovation Funding Authority (STDF) in cooperation with The Egyptian Knowledge Bank (EKB).
The authors declare that they have no competing interest.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Abou Elmaaty, T., Abd Elsalam, S., Helal, S. et al. In situ anchoring iron oxide nanoparticles onto polyester/disperse dye for production of multifunctional fabrics. Fash Text 10, 41 (2023). https://doi.org/10.1186/s40691-023-00362-8